Vertical field effect tunneling transistor based on ... PDF file Vertical field effect tunneling...
Embed Size (px)
Transcript of Vertical field effect tunneling transistor based on ... PDF file Vertical field effect tunneling...
This content has been downloaded from IOPscience. Please scroll down to see the full text.
IP Address: 18.104.22.168
This content was downloaded on 09/11/2015 at 04:36
Please note that terms and conditions apply.
Vertical field effect tunneling transistor based on graphene-ultrathin Si nanomembrane
View the table of contents for this issue, or go to the journal homepage for more
2015 2D Mater. 2 044006
Home Search Collections Journals About Contact us My IOPscience
iopscience.iop.org/page/terms http://iopscience.iop.org/2053-1583/2/4 http://iopscience.iop.org/2053-1583 http://iopscience.iop.org/ http://iopscience.iop.org/search http://iopscience.iop.org/collections http://iopscience.iop.org/journals http://iopscience.iop.org/page/aboutioppublishing http://iopscience.iop.org/contact http://iopscience.iop.org/myiopscience
2DMater. 2 (2015) 044006 doi:10.1088/2053-1583/2/4/044006
Vertical field effect tunneling transistor based on graphene-ultrathin Si nanomembrane heterostructures
TanmoyDas,Houk Jang, Jae Bok Lee,HyunwooChu, SeongDaeKim and Jong-HyunAhn School of Electrical and Electronic Engineering, Yonsei University, Seoul, 120-749, Korea
Keywords: graphene, Si nanomembrane, tunneling transistor, heterostructures
Abstract Graphene-based heterostructured vertical transistors have attracted a great deal of research interest. Hereinwe propose a Si-based technology platform for creating graphene/ultrathin semiconductor/ metal (GSM) junctions, which can be applied to large-scale and low-power electronics compatible with a variety of substrates.We fabricated graphene/Si nanomembrane (NM)/metal vertical heterostructures by using a dry transfer technique to transfer SiNMs onto chemical vapor deposition- grown graphene layers. The resulting van derWaals interfaces between graphene and p-SiNMs exhibited nearly ideal Schottky barrier behavior. Due to the low density of states of graphene, the graphene/SiNMSchottky barrier height can bemodulated bymodulating the band profile in the channel region, yieldingwell-defined currentmodulation.We obtained amaximum current on/off ratio (Ion/Ioff) of up to∼10
3, with a current density of 102 A cm−2.We also observed significant dependence of Schottky barrier heightΔjb on the thickness of the SiNMs.We confirmed that the transport in these devices is dominated by the effects of the graphene/SiNMSchottky barrier.
Recent rapid progress in basic science and applications of graphene has opened the way for materials just one atom thick to be used in future electronics, including devices with new structures. Graphene’s unique physi- cal properties, such as its two-dimensional structure, high carriermobility, and low density of states, make it attractive for high-speed electronic devices [1–5]. However, graphene-based field-effect transistors can- not be completely switched off due to the lack of an intrinsic band gap in graphene; hence, they are inappropriate for digital logic applications [6, 7]. On the other hand, heterostructures based on graphene and other two-dimensional crystals have been demon- strated that can be assembled into three-dimensional stacks with atomic-layer precision; these have shown a variety of fascinating physical phenomena and have aroused immense interest in demonstrating a proto- typefield-effect tunneling transistor, which is regarded as a candidate technology to replace complementary metal-oxide semiconductor technology [6, 8, 9]. In particular, various vertically layered heterostructures based on work function tunability of graphene have
been studied recently, such as graphene-based tunnel- ing transistors (called barristors) and vertical field- effect transistors (VFETs); these have shown improved Ion/Ioff characteristics compared to planar graphene field-effect devices [10, 11]. The demonstration of such vertically stacked heterostructures has opened up potential high-performance applications in tunneling transistors, photovoltaic cells, and flexible devices based on two-dimensional (2D) materials. A broad range of possible materials can be incorporated into such stacks by weak van der Waals forces to create novel highly tailored heterostructures [3, 15, 16]. To create VFET heterojunctions, various kinds of 2D barrier materials have been considered, such as exfoliated hexagonal boron nitride, molybdenum disulfide, and tungsten disulfide, but critical challenges still remain forwafer-scale integration [12, 13, 17].
On the other hand, single-crystal Si NMs, formed in large sheets with precisely defined thicknesses com- parable to 2D materials, offer unique advantages over other transition-metal dichalcogenides. Si NMs are compatible with established semiconductor techni- ques, and can have exceptional material quality, com- positional purity, and high uniformity, leading to
2 July 2015
ACCEPTED FOR PUBLICATION
3 September 2015
© 2015 IOPPublishing Ltd
http://dx.doi.org/10.1088/2053-1583/2/4/044006 mailto:email@example.com http://crossmark.crossref.org/dialog/?doi=10.1088/2053-1583/2/4/044006&domain=pdf&date_stamp=2015-11-02 http://crossmark.crossref.org/dialog/?doi=10.1088/2053-1583/2/4/044006&domain=pdf&date_stamp=2015-11-02
straightforward paths for wide-scale integration into existing Si-based technology platforms. Transferrable single-crystal Si NMs are often more suitable than other 2D materials for use as active materials in flex- ible electronics due to their material uniformity, mechanical flexibility and durability, electrical proper- ties equivalent to their bulk counterparts, easy hand- ling and processing, and low cost [18–22]. There is a broad range of electronics applications in which mechanically flexible materials with higher speed are needed; these applications include flexible electronics and optoelectronics, including transparent electro- nics. Because the thickness of Si NMs is controllable, their use may allow this range of applications to be extended.
Herein we describe a new generation of vertical tunneling transistors in which ultrathin Si NMs serve as an ultrathin 2D barrier material between chemical vapor deposition (CVD)-grown graphene and a metal electrode. By utilizing the Schottky barrier height between graphene and Si NMs in ultrathin Si-based tunneling transistors, the device characteristics can be improved considerably, to the extent that the resulting device can satisfy the requirements for next-genera- tion electronic devices. Ultrathin Si NMs offer distinct advantages over other 2D materials, including their chemical stability and moderate band gaps. Addition- ally, the use of the dry transfer technique with Si NMs can produce a clean interface between graphene and Si NMs that exhibits nearly ideal Schottky diode beha- vior, thereby yielding strong current rectification.
Figure 1(a) schematically illustrates a typical vertical transistor of our design. The fabrication techniques for the vertical transistor are schematically illustrated in the methods section. Briefly, monolayer graphene was first grown by CVD and transferred onto a silicon wafer with a SiO2 layer 285 nm thick . Then, the transferred graphene layer was patterned by photo- lithography and oxygen plasma etching into strips
25 μm wide and 100 μm long to define the drain electrode. SiNMsof various thicknesseswere prepared from commercial silicon-on-insulator (SOI)wafers, as previously reported . Before transferring a Si NM onto the graphene, the native oxide on the exposed Si substrate was carefully removed by additional wet etching, and the Si surface was then passivated by hydrogen treatment. Then, the Si NM surface was treated with a UV ozone treatment to form a thin surface passivation layer, and the passivated Si NM was stacked onto the graphene contact by means of a dry transfer technique . The top metal electrode was formed by electron-beam lithography and thermal evaporation of Ni/Au (20/30 nm) onto the Si NMs to overlap the bottom graphene electrode. We studied more than a dozen graphene/Si NM heterostructures with a diverse range of thicknesses from 8 to 100 nm, and observed qualitatively similar behavior for each batch of devices.
3. Results and discussion
Figure 1(b) shows an optical image of a fabricated device. The 25 μm strip of monolayer graphene is located inside the dotted lines. The total channel area is defined by the area of overlap between the graphene and the top metal electrode. A cross-sectional trans- mission electron microscope (TEM) image showing the region from the top drain electrode to the bottom source electrode was taken to investigate the overall integration of the graphene/Si NM/top electrode vertical stack, and to study the interface (figure 1(c)). The well-optimized transfer process including surface pre-treatment produced clean interfaces between graphene and Si, free from native oxide or other contamination layers. In a larger-area TEM image of unoptimized Si NMs transferred onto graphene, contamination was observed, as was native oxide between the graphene and Si (supplementary informa- tion). Reducing damage to the silicon substrate during the wet etching of silicon oxide was identified as a key factor in producing atomically clean interfaces.
Figure 1.Graphene/SiNMheterostructure layout: (a)Three-dimensional schematic illustration of the vertically stacked graphene/Si NM/metal transistor. (b)Optical im